Review: environmental friendly lead-free piezoelectric materials
Lead zirconate titanate (PZT) based piezoelectric materials are well known for their excellent piezoelectric properties. However, considering the toxicity of lead and its compounds, there is a general awareness for the development of environmental friendly lead-free materials as evidenced from the legislation passed by the European Union in this effect. Several classes of materials are now being considered as potentially attractive alternatives to PZTs for specific applications. In this paper, attempts have been made to review the recent developments on lead-free piezo materials emphasizing on their preparation, structure–property correlation, etc. In this context, perovskite systems such as bismuth sodium titanate, alkali niobates (ANbO3), etc. and non-perovskites such as bismuth layer-structured ferroelectrics are reviewed in detail. From the above study, it is concluded that some lead-free compositions show stable piezoelectric responses even though they do not match the overall performance of PZT. This has been the stimulant for growing research on this subject. This topic is of current interest to the researchers worldwide as evidenced from the large number of research publications. This has motivated us to come out with a review article with a view that it would give further impetus to the researchers already working in this area and also draw the attention of the others.
Piezoelectricity (pressure electricity) was discovered by Nobel laureates Pierre and Jacques Curie in 1880  during their study of the effects of pressure on the generation of electrical charge by crystals such as quartz, tourmaline, and Rochelle salt. In fact, the development of an electrical charge under the application of mechanical pressure or vice versa is referred to as the piezoelectric effect. Low piezo-electricity is the main drawback of the natural piezoelectric materials. A major break through came with the discovery of PZT and BaTiO3 in the 1950s [2, 3] and the family of these materials exhibited very high dielectric and piezoelectric properties. To date, PZT is one of the most widely exploited and extensively used piezoelectric materials, having secured a permanent place in the field of material science and engineering. They are widely used as sensor and actuator devices [4, 5, 6, 7], multilayered capacitors, as hydrophones, etc. with an estimated market of tens of billions of dollars worldwide. However, lead oxide, which is a component of PZT, is highly toxic and its toxicity is further enhanced due to its volatilization at high temperature particularly during calcination and sintering causing environmental pollution .
Properties of some selected lead-free compositions
(Na0.5Bi0.5)0.92Ba0.08TiO3 + xNb2O5
BNT–BT–CeO2 + La2O3
(Na0.5Bi0.5)0.94–6BaTiO3 + 0.5 mol% CeO2 + 0.5 mol% La2O3
(Na0.5Bi0.5)0.92–Ba0.08TiO3 + x mol% MnCO3
Bi0.5(Na0.84K0.16)0.5TiO3 + xSrTiO3
AE = Mg, Ca, Sr, Ba
The large piezoelectric response of PZT results from two factors. Primarily, the stereo-chemical activity of the 6s2 lone pair on the lead ion causes large structural distortions from the cubic perovskite phase that results in strong coupling between the electronic and structural degrees of freedom . Bi-based compounds have similar or larger levels of ion off centering than Pb-based compounds, driven by the stereo chemically active 6s2 lone pairs on the Bi3+ ion. This leads to large ferroelectric polarizations. In most common ferroelectrics, ion off centering is mainly contributed by the B-site cations to the ferroelectricity so as to increase the chemical bonding between their valence d orbital and the surrounding oxygen 2p orbital (second-order Jahn Teller, SOJT) effect . Bismuth is non-toxic in its oxide forms; indeed, the active ingredient of a popular antacid is bismuth salicylate. Some of the toxic effects of lead and its hazardous consequences on health are discussed in the next section.
Toxic effects of lead
Symptoms and signs of lead poisoning 
Gingival lead line
Peripheral neuropathy (motor)
Lead has three important biochemical properties that contribute to its toxic effects on humans. First, lead being an electropositive metal has high affinity for enzymes, which are essential for the synthesis of hemoglobin. Second, divalent lead acts in a manner similar to calcium inhibiting mitochondrial oxidative phosphorylation thus reducing the intelligence quotient. Lead can also affect the genetic transcription of DNA by interaction with nucleic acid binding proteins . The most important initial aspect of management of lead poisoning is the removal of the patient from the source of exposure  and second by using chelating agents (EDTA) that form complexes with lead and hence are excreted out [22, 23, 24, 25].
In this paper, overview of current developments in various lead-free piezoelectric ceramics, effects of various dopants to enhance the piezo properties were presented.
Perovskite-structured lead-free ferroelectrics
The perovskite-type (ABO3) ferroelectrics such as BaTiO3 (BT), (Bi0.5Na0.5)TiO3 (BNT), KNbO3, NaTaO3, etc. are well-known lead-free piezoelectric materials. These ceramics show relatively large piezoelectric constant. However, the main drawbacks generally are low Curie temperatures (Tc), difficulties in poling treatments and/or low relative densities .
Barium titanate, BaTiO3 (BT) is one of the perovskites discovered very early. It has a relatively high electromechanical coupling factor (k33) and has been partially used for piezoelectric applications such as sonar although its main use is for capacitor applications. It has the advantage of easy manufacture by various ceramic techniques. BT has a low Curie temperature (Tc = 120 °C) causing the working temperature range of this ceramic narrow for actual piezoelectric applications. To increase the Tc of BaTiO3-based ceramics, a binary system of BaTiO3–(Bi0.5K0.5)TiO3 (BKT) was investigated. The Tc of BKT was reported to be about 380 °C .
BaTiO3 and (Bi0.5K0.5)TiO3 system
(Bi1/2Na1/2)TiO3 (BNT) is one of the important lead-free piezoelectric materials with perovskite structure discovered by Smolenskii et al. . As (Bi1/2Na1/2)TiO3 composition exhibits strong ferroelectric properties of a large remnant polarization, Pr = 38 μC/cm2 and high Curie temperature, Tc = 320 °C, it has been considered for lead-free piezoelectric ceramics as an alternative to the widely used lead-based piezoelectric materials . The main drawback of this material is its high conductivity, consequently giving problems in the poling process. In addition, BNT ceramics need high sintering temperature (>1200 °C) to obtain the dense body. Thus BNT is considered to be a promising candidate for lead-free piezoelectric ceramics with balanced ferroelectric properties.
Effect of dopants on BNT ceramics
Effect of La2O3
Effect of dopants on BNT system
Tan δ (%)
x = (0–0.6 mol%)
x = 1
x = 1.72
x = 2
x = 3
x = 0.01
x = 0.02
x = 0.03
x = 0.04
x = 0.05
Effect of NaNbO3
Li et al. prepared lead-free bismuth sodium titanate-sodium niobate (BNT-NN), [Na0.5(1+x)Bi0.5(1–x)](Ti(1–x)–Nbx)O3 ceramics using conventional ceramic technique . They concluded that d33 increases from 64 to 88 pC/N for 2 mol% of NaNbO3 and then decreases gradually. However, the dielectric constant increases gradually with increase in NaNbO3 content. This is attributed to the co-effect of the soft additive Nb5+ ion doping at B-site and hard additive Na+ ion doping at A-site. However, with further increasing the doping content of NaNbO3 (x = 0.03–0.05), the piezoelectric properties decreased, which may be the reason for the dominant doping of Na+ ion shown in Table 5 .
Effect of BaTiO3
Properties of BNT-BT system
Effect of Bi2O3 · Sc2O3
Properties of (1–x)(Bi0.5Na0.5)TiO3–x(Bi2O3 · Sc2O3)0.5 system
Tan δ (%)
Effect of La, Nb, Co
Effect of dopants on BNT–BT system
Tan δ (%)
(Na0.5Bi0.5)0.92Ba0.08TiO3 + xNb2O5 (NBBT83)
(Na0.5Bi0.5)0.92–xBa0.08TiO3 + xCo2O3 (NBBT84)
(Na0.5Bi0.5)TiO3–6BaTiO3 + La(BNBT6) + La
(Na0.5Bi0.5)TiO3–6BaTiO3 + Nb (BNBT6) + Nb
(Na0.5Bi0.5)TiO3–6BaTiO3 + La–Co (BNBT6) + La–Co
(Na0.5Bi0.5)TiO3–6BaTiO3 + La–Nb (BNBT6) + La–Nb
(Na0.5Bi0.5)TiO3–6BaTiO3 + Co (BNBT6) + Co
(Na0.5Bi0.5)0.94–6BaTiO3 + 0.5 mol% CeO2 + 0.25 mol% La2O3
(Na0.5Bi0.5)0.94–6BaTiO3 + 0.5 mol% CeO2 + 0.5 mol% La2O3
(Na0.5Bi0.5)0.94–6BaTiO3 + 0.5 mol% CeO2 + 0.75 mol% La2O3
(Na0.5Bi0.5)0.92–Ba0.08TiO3 + x mol% MnCO3
Effect of La2O3 and CeO2
Some further enhancement in these properties was reported by adding La2O3 and CeO2. From Table 8, it could be concluded that addition of equal amount of 0.5 mol% CeO2 together with 0.5 mol% of La2O3 increases d33 value from 129 to 162 pC/N. The dielectric constant also increases from 625 to 831. It has been reported that CeO2 has the dual effect of improving the piezoelectric properties of BNBT-6 ceramics and decreasing the dissipation factor. Ce3+ with a radius of 1.18 Å occupies the A-site as Ba2+ in the BNBT lattice and functions as a donor leading to some A-site vacancies. Meanwhile, Ce4+ with a radius of 0.94 Å goes into the Ti4+ site and changes the space charge. La2O3 is a typical soft additive for PZT ceramic occupying a Bi3+ site or a Ba2+ site .
Effect of Mn
The maximum value of the piezoelectric constant was 160 pC/N for BNBT doped with 0.56 mol% Mn at room temperature . From the table, it can also be seen that with increasing the amount of the dopant, the Tc decreases rapidly. When the amount of Mn is lower than 0.56 mol%, the increase in piezoelectric properties is partly due to the decrease of tetragonality of BNBT. Additionally, the incorporation of smaller cations in a normal perovskite structure causes the slack of lattice and enhances the motion of 90° domains. When the amount of Mn is over 2.6 mol%, it is supersaturated in the lattice of BNBT and the excess of Mn ions are accumulated in the grain boundaries, resulting in the pinning effect of the domain. Ichinose and Udagawa have studied that the piezoelectric property of (Bi0.5Na0.5)0.87(Sr0.5Ca0.5)0.13TiO3 system was close to MPB composition from the view point of lead-free piezoelectric materials. MnO was added up to 1 wt% to this system in order to improve the electromechanical and mechanical properties of the system .
A number of lead-free piezoelectric ceramic materials have been developed to replace the PZT-based ceramics for environmental protection . However, BNT still cannot replace PZT-based ceramics due to large coercive field and high conductivity. Recently, many researchers have investigated the effects of small amount of dopants (cation modifications) into BNT ceramics such as Ba, Pb, Ca, Sr, Ce, Se, NaNbO3, etc. and successfully overcome the problems mentioned above.
Jhang et al. investigated the microstructure and electrical properties of Bi-compensated BNT–BKT ceramics sintered at 1110–1170 °C [58, 59]. Increasing sintering temperatures enhanced the grain growth, densification, and improvement of piezoelectric and ferroelectric properties. However, as the temperature was increased to 1170 °C, the piezoelectric properties deteriorated seriously. An MPB-like phase transition from tetragonal to rhombohedral symmetry was found in BNKT20 and BNKT22 specimens sintered between 1150 and 1170 °C. Enhanced electrical properties were obtained for the BNKT22 samples sintered at an optimal temperature of 1150 °C, in which d33, Pr, and K were 192 pC/N, 19.5 μC/cm2, and 1007, respectively.
Effect of Strontium (Sr)
Effect of NaNbO3
Properties of Bi(Na,K,Li)TiO3 system
Properties of Bi(Na,K,Li)TiO3–BaTiO3 system
Li et al. also prepared (1–5x)BNT–4xBNT–xBT ceramic by conventional ceramic fabrication technique . The piezoelectric and ferroelectric properties of these ceramics were studied. They were of the conclusion that the piezoelectric constant d33 attains a maximum value of 149 pC/N at x = 0.03. This property demonstrates that the compositions near the MPB have relatively high piezoelectric activities.
Lead-free piezoelectric ceramic 0.90(Bi0.5Na0.5)TiO3–0.05(Bi0.5K0.5)TiO3–0.05BaTiO3 (abbreviated as BNT–BKT–BT5) has been used recently as the driving element in a cymbal actuator with titanium end caps. It was found that the lead-free ceramic cymbal actuator has reasonable piezoelectric coefficients and low density. Hence its performance was comparable to those fabricated using hard PZT ceramic .
Matthias discovered ferroelectricity in potassium niobate, KNbO3 . Alternative lead-free materials of the perovskite family with the general formula, ANbO3 (A = alkali metal) were proposed by researchers in the 1950s and 1960s . KNbO3 (KN) has an orthorhombic symmetry at room temperature, and KN single crystals are known to have high piezoelectric activities. It is known that KNbO3 and related compounds show a high Curie temperature (Tc = 435 °C) and good piezoelectric properties.
Park et al.  elaborately studied the effect of CuO on KNN ceramics. They observed that addition of CuO decreases the sintering temperature of KNN below 1000 °C in order to prevent the Na2O evaporation and to eventually improve the piezoelectric properties by increasing their polling efficiency. When a small amount of CuO was added, a dense microstructure with increased grain size was developed. Liquid-phase sintering was considered to have been responsible for the development of the dense microstructure. The Cu2+ ion replaced the Nb5+ ion and produced an oxygen vacancy to maintain the charge neutrality. A defect dipole consisting of the Cu2+ ion and oxygen vacancy provided the pinning effect, which eventually transformed the NKN ceramics into the hard materials. The Curie temperature and Ec were slightly increased with CuO addition.
Bernard et al.  found that the densification of KNN ceramics can be improved by the addition of a small amount (from 0.5 to 4 mass%) germanate, which melts at around 700 °C. Germanate-modified KNN ceramics can be sintered to high density (95.6% TD) at 1000 °C without degrading the piezoelectric properties.
Comparison of properties of alkali niobates obtained by different processing methods
Air-sintered (Jaeger–Egerton) K0.5Na0.5NbO3
Air-sintered (Kosec) K0.5Na0.5NbO3
Air-sintered H. (Birol) K0.5Na0.5NbO3
Hot-pressed (Jaeger–Egerton) K0.5Na0.5NbO3
Hot-forged (Schultze) K0.5Na0.5NbO3 + 4 mol% Ba
Reactive grain growth (Saito et al.)
Effect of dopants on KNN-based ceramics
Potassium sodium niobate is a promising lead-free material with low dielectric constant and high electromechanical coupling coefficient. However, it is difficult to prepare KNN ceramics with high density by conventional sintering technique. Sintering may be activated by the addition of Nb5+ or Mg2+ ions in the crystal lattice thereby producing high-density sample [81, 82, 83, 84].
(i) Effect of LiTaO3and LiSbO3: The effect of incorporated LiTaO3 on the structure, phase transition behavior and electrical properties of the KNN system have been studied [85, 86, 87, 88, 89, 90]. It was established that Ta substitution for Nb, changes the properties of KNbO3 and the authors also demonstrated that small amounts of Ta for Nb could enhance the piezoelectric properties of KNN ceramics [72, 91]. Saito et al.  also developed a lead-free system containing a blend of alkaline niobate (Tc = 415 °C) based solid solution with LiTaO3 (Tc = 615 °C). This system gave good piezoelectric response with a d33 of 230 pC/N. Addition of LiSbO3 to the above system increased the d33 to 373 pC/N . Many authors have been studied the effect of LiSbO3 (LS) on pure KNN ceramics [93, 94, 95]. Yang et al.  studied the effect of LS on pure KNN ceramics and reported that increasing the LS content, the d33 and kp values of the ceramics initially increased, and then began to decrease at higher LS concentration. In addition, dielectric study revealed that Tc shifted toward the lower temperature regions and a normal ferroelectric KNN-based ceramics changed to relaxor ferroelectric by increasing LS content. The KNN–LS ceramics are promising lead-free piezoelectric materials for electromechanical transducer applications. Effect of other ions such as Ag, Nb, Ta, Bi, Cu, Ca, etc. and combination two or three cations on KNN–LS ceramics were also studied by many authors [96, 97, 98, 99, 100, 101, 102, 103, 104, 105, 106, 107, 108] and promising results were reported. Wang et al. reported that addition of Ag in KNN–LiTaO3 ceramics increases the Curie temperature (Tc = 438 °C) and piezoelectric properties (d33 = 252 pC/N) of the ceramic by normal sintering technique .
(ii) Effect of alkaline earth ions: The effect of low amount of alkaline earth dopants, (0.5 at.%) Mg2+, Ca2+, Sr2+, and Ba2+ on KNN solid solution synthesis, sinterability, and functional response of corresponding ceramics was also studied by different authors [110, 111, 112, 113]. They were chosen on the basis of the similarity of their ionic radii to those of K+ and Na+. Chang et al.  observed that adding Ca2+ and Sr2+ to KNN can make the cell parameters increase, promote densification, decrease the phase transition temperatures, and improve the electrical properties. However, adding Mg2+ to KNN can lower the cell parameters and density, increase Tc, and seriously deteriorate the electrical properties. Adding Ba2+ to KNN can increase the cell parameters, decrease the density, decrease the phase transition temperatures, and also significantly deteriorate electrical properties.
(iii) Effect of BaTiO3: BaTiO3 is one of the typical ferroelectric materials showing large piezoelectricity, but its low Tc limits the application. However, by the addition of BaTiO3 to Na1–xKxNbO3, it could be anticipated that the solid solution would show a relatively high Tc with piezoelectricity comparable to BaTiO3 [115, 116]..
Non-perovskite structured lead-free ferroelectrics
Bismuth layer-structured ferroelectrics
Aurivillius type structure oxides with general formula Bi2An−1BnO3n+3, which consist of n-perovskite layers [An−1BnO3n+1]2− sandwiched between bismuth oxygen sheets [Bi2O2]2+ come under BLSF. The perovskite layer can be a one, two, three, or more perovskite unit thick. Each of these results in a separate structure type, but has the perovskite layer-bismuth oxide layer alteration . Possible substitutions into Bi-site of bismuth oxide layer by other p-cations that have a stereo-chemical active lone pair of electrons, such as Pb2+, Sb3+, and Te4+ have been reported. Bi3NbTiO9 is an example of such compound because of its high Tc (914 °C), however it posses very weak piezoelectric effects. The maximum d33 reported for any of these layer structure compositions is 25 pC/N . The family of BLSF is very attractive from the viewpoint of their applications as electronic materials such as dielectrics, piezoelectric, and/or pyroelectric. BLSF are characterized by their low dielectric constant, high Curie temperature (Tc), and large anisotropy in the electromechanical coupling factor. Therefore, the BLSF ceramics are seen as superior candidates for lead-free piezoelectric applications for high Tc piezoelectric sensors, filters, resonators, and/or pyroelectric sensors with large figures of merit .
Bi4Ti3O12-based BLSF system
Bismuth titanate, Bi4Ti3O12, is a typical well-known BLSF. Concerning the anisotropy, Cross and Pohanka  reported that BiT single crystal has good piezoelectricity. However, it is difficult to measure piezoelectric properties on the BiT single crystal because of its thin structure. On the other hand, fully reliable piezoelectric properties of BiT ceramics have not been reported because of some problems such as the low resistivity and the large coercive field. To solve these problems, Nb5+ and V5+ ions were doped into BiT ceramic to obtain higher resistivity .
Bi3TiTaO9-based BLSF system
Bismuth layer-structured ferroelectrics of the type, Bi3TiNbO9 and CaBi2Ta2O9, possess very high Tc above 800 °C . These data suggest that high mechanical quality factor (Qm) is obtained by BLSF materials with high Tc making them suitable for electromechanical transducer required to sense strains, vibrations, and noise under severe thermal conditions. By this concept, dielectric, ferroelectric, and piezoelectric properties of Bi3TiTaO9 (BTT) based solid solution system with a high Tc were also investigated . The authors have studied that in the Sr-site substituted compositions, there is a variation of the phase transition temperature with the ionic radius size and the amount of modifier, but no extra peaks in dielectric constant have been observed .
Non-perovskites with lead-free tungsten-bronze structure
A number of ferroelectrics of potential commercial importance have the potassium tungsten-bronze AxB2O6 structure. Some examples are BaNb2O6, SrNb2O6, SrxBa1–xNb2O6, AB2O6 type, etc. Piezoelectric ceramics with tungsten-bronze structure are potentially served as sensors in sensing patches, single crystals for electro-optic uses, etc. Matsuo et al. studied the effect of doping Sr2–xCaxNaNb5O15 with La2O3 and concluded that a dielectric constant of 1662, Curie temperature of 298 °C, spontaneous polarization of 10.7 μC/cm2 and piezoelectric constant of 138 pC/N was obtained, respectively. The piezoelectric properties of the SCNN-based ceramics indicate that they are good candidates for sensor applications [120, 121, 122, 123]. The study investigating the electrical properties of dense lead-free piezoelectric ceramics in the (1–x)Sr2NaNb5O15–xCa2NaNb5O15 (SCNN) system with x ranging from 0.05 to 0.35 has also been reported. Ferroelectric and piezoelectric properties of SCNN greatly depended on the Ca content. The composition with x = 0.15 exhibited piezoelectric constant of d33 = 96 pC/N. This study apparently indicates that lead-free SCNN piezoelectric ceramics have potential for electromechanical applications.
Processing methodology of piezoelectric ceramics
The fabrication of most bulk piezoelectric ceramics starts with powder preparation. The powder is then pressed to the required shapes and sizes, and the green shapes are in turn processed to mechanically strong and dense ceramics. The next steps are machining, electroding, and poling-application of a DC field to orient the dipoles and induce piezoelectricity.
The most common powder preparation is the mixed oxide route. In this process, powder is prepared from the appropriate stoichiometric mixture of the constituent oxides. Mixing of the powders is done by dry ball-milling or wet ball-milling, both methods having advantages and disadvantages: wet ball-milling is faster than dry-milling; however, the disadvantage is the added step of liquid removal. A vibratory mill may be used rather than a conventional ball mill.
Depending on application, various dopants are used to tailor the properties of interest. A-site additives tend to lower the dissipation factor, which affects heat generation, but also lower the piezoelectric coefficients; for this reason, they are mostly used in ultrasonic and other high frequency applications. B-site dopants increase the piezoelectric coefficients but also increase the dielectric constant and loss. They are utilized as actuators in vibration and noise control, benders, optical positioning application, etc.
Apart from the conventional “mixed oxide” method, lead-free piezo-materials are also prepared by various chemical routes such as by sol–gel, wet-chemical route, co-precipitation, etc., similar to the processing methods followed for the synthesis of PZTs. The calcination step is a very crucial step in the processing of PZT ceramics. During calcination organics, water or other volatiles are removed and formation of required phases takes place. The crystal structure is confirmed by X-ray diffraction analysis. After calcination, binder was added to the powder and compacted into pellets. They are then sintered at temperatures varying between 1100 and 1200 °C. Electrodes (conducting silver paste) are applied and a strong DC field is used to orient the domains in the polycrystalline ceramic and the dielectric and piezoelectric properties were measured after poling.
This processing technique present many uncertainties—one problem often encountered is the deviation from stoichiometry. Also, the piezoelectric and dielectric properties generally suffer if there is any lack of homogeneity due to poor mixing. It is important then that the constituent oxides be intimately mixed. More information on the preparation of piezoelectric ceramics can be found in Jaffe et al. , and Moulson and Herbert  among others. Other processing methods including hydrothermal processing and co-precipitation methods are described in references [125, 126, 127, 128, 129].
BNT is considered to an excellent candidate for lead-free piezoelectric ceramics with a high Tc of 320 °C, as well as relatively large remnant polarization, Pr of 38 μC/cm2 and coercive field, Ec of 73 kV/cm. Still BNT cannot replace PZT due to its large coercive field and high conductivity. Hence researchers have investigated many dopants into BNT ceramics to solve these problems.
In addition to that, scientists have developed multicomponent systems, which have higher piezoelectric properties than binary systems. For example, BaTiO3, KNbO3 combined with a rhombohedral compound to yield a high activity MPB system.
The density of lead-free piezoelectric materials are approximately half of the density of PZTs; therefore, the effective specific piezo properties per unit weight of lead-free materials are double their actual values when these materials have to be compared with PZTs. For example, a d33 value of 150 pC/N of a lead-free material is nearly equivalent to 280–300 pC/N of PZT material.
Lead-free materials like BNT, NaNbO3, KNbO3, etc. were also developed simultaneously along with PZT in the 1950s. But due to the excellent piezoelectric properties exhibited by the PZTs, the researchers were preferred to work on the PZT system; hence, not much work was done on lead-free materials. Even though the initial results on PZT system showed lower piezo properties, the values were largely enhanced after the discovery of MPB, addition of suitable dopants, etc., studied systematically. A similar systematic approach may be required for the enhancement of piezo properties of lead-free materials at least very near to the level of PZTs.
Lead-free piezoelectric materials with excellent dielectric and piezoelectric properties belonging to the perovskite ferroelectric and bismuth layer-structured (BLSF) ceramics were investigated as superior candidates to reduce environmental damages. The families of sodium potassium niobate and bismuth sodium titanate that come under the perovskite type ceramics seem to be suitable for actuator and high power applications with a piezoelectric constant, d33 > 150 pC/N and a high Curie Temperature, Tc > 200 °C. For high temperature applications (>600 °C), bismuth-layered compounds show good stability of properties and hence they serve as excellent candidates for piezoelectric sensors. In order to replace PZT systems, it is necessary that special features of each lead-free material correspond to required piezoelectric properties for each application.
The author expresses his sincere gratitude to Mr. M.K. Sridhar, Head, Materials Science Division and Dr. A. R. Upadhya, Director, NAL for their support and encouragement during the course of the study. The author also thanks to M. Sunitha and Benudhar Sahoo for their help in the preparation of the manuscript.
- 1.Curie J, Curie P (1880) Bulletin de la Societe Mineralogique de France 3:90Google Scholar
- 2.Jaffe B, Jaffe H, Cook WR (1971) Piezoelectric ceramics, 1st edn. Academic Press, LondonGoogle Scholar
- 3.Haertling GH (1991) In: Buchanan RC (ed) Piezoelectric and electro-optic ceramics in ceramic materials for electronics, 2nd edn. Marcel Dekker, New YorkGoogle Scholar
- 4.Uchino K (1993) Mater Res Bull 18:42Google Scholar
- 5.Newnham RE (1998) Functional composites for sensors and actuators: smart materials. The Pennsylvania Academy of Science, PA, USAGoogle Scholar
- 19.Control of Lead at Work Regulations (1998) London: The Stationery Office LtdGoogle Scholar
- 22.Kety SS (1942) J Biol Chem 142:181Google Scholar
- 29.Smolenskii GA, Isupov VA, Agranovskaya AI, Krainik NN (1961) Sov Phys Solid State 2:2651Google Scholar
- 36.Peng CE (2006) Master’s degree thesis, Tsinghua University, China, pp 66–75Google Scholar
- 47.Takenaka T, Sakata K, Toda K (1990) Ferroelectrics 106:375Google Scholar
- 56.Ichinose N, Udagawa K (1995) Ferroelectrics 169:317Google Scholar
- 57.Kusumoto K, Ceramics Research Institute, National Institute of Advanced Industrial Science and Technology (AAST), Nagoya, JapanGoogle Scholar
- 71.Jona F, Shirane G (1993) Ferroelectric crystals. Dover Publications Inc., New York, p 221Google Scholar
- 73.Matsubara M, Kikuta K, Hirano S (2005) J App Phys 97:114Google Scholar
- 120.Huseyin Y, Susan T, Gary M (2003) J Electro Ceram 11:217Google Scholar
- 121.Matsuo K, Xie RJ, Akimune Y, Sugiyama T (2002) J Ceram Soc Jpn 110:491Google Scholar
- 123.Patro PK, Kulkarni AR, Gupta SM, Harendranath CS (2006) In: Kharat DK (ed) National seminar on advances in electroceramics (NSAE-2006), Armament Research & Development Establishment, Pune, India, pp 146–153Google Scholar
- 124.Moulson AJ, Herbert JM (1992) Electroceramics: materials, properties, applications. Chapman and Hall, LondonGoogle Scholar
- 126.Measurement of properties of piezoelectric ceramics, Sensor Technology Limited (1991) Manufacturer Handbook, BM91-309Google Scholar
- 128.Ounaies Z (1995) Sol–gel and microwave processing of PZT materials for sensor and actuator application. The Pennsylvania State University, PA, USAGoogle Scholar
- 129.Levinson LM (1998) Electronic ceramics: properties, devices and applications. General Electric Company, New YorkGoogle Scholar